The effect of high vacuum on the mechanical properties and bioactivity of collagen fibril matrices
© Anderton et al.; licensee Springer. 2013
Received: 6 December 2012
Accepted: 17 January 2013
Published: 17 January 2013
The extracellular matrix (ECM) environment plays a critical role in organism development and disease. Surface sensitive microscopy techniques for studying the structural and chemical properties of ECMs are often performed in high vacuum (HV) environments. In this report, we examine the affect HV conditions have on the bioactivity and mechanical properties of type I collagen fibrillar matrices. We find that HV exposure has an unappreciable affect on the cell spreading response and mechanical properties of these collagen fibril matrices. Conversely, low vacuum environments cause fibrils to become mechanically rigid as indicated by force microscopy, resulting in greater cell spreading. Time-of-flight secondary ion mass spectrometry results show no noticeable spectral differences between HV-treated and dehydrated matrices. While previous reports have shown that HV can denature proteins in monolayers, these observations indicate that HV-exposure does not mechanically or biochemically alter collagen in its supramolecular configuration. These results may have implication for complex ECM matrices such as decellularized scaffolds.
Cellular interactions with the extracellular matrix (ECM) initiate an array of biophysical and biochemical signals that drive biological processes ranging from embryonic development to cancer progression [1–4]. In addition to receptor-mediated interactions between cells and the ECM [5, 6], the mechanical environment that cells experience can exert strong influences on inter- and intracellular signaling and cell responses, and is likely critical to migration, differentiation, and development [4, 7–10]. Elucidating the structural, mechanical, and chemical environment that the ECM presents to cells can be challenging. There has been a growing effort to employ a variety of surface sensitive microscopy techniques to measure the physicochemical properties of ECMs [11–16].
Recently, a number of reports have analyzed decellularized tissues and ECMs created by cells in vitro using electron, ion, and x-ray bombardment induced ionization microscopy methods, which are performed under high vacuum (HV) [13–15, 17–22]. The use of scanning electron microscopy (SEM), for example, is commonplace for obtaining structural information of supramolecular ECM systems [13, 17, 18, 20], but methods for accessing information about the chemical environment that the ECM provides to cells has been more elusive. Time-of-flight secondary ion mass spectrometry (ToF-SIMS) is one such technique that can provide chemical information about the surface of the material being analyzed. The ToF-SIMS sampling depth, when operated in a so-called static mode, is approximately 1 nm to 2 nm, rendering it ideal for determining the surface composition of complex protein samples [14, 23–26]. ToF-SIMS data are conducive to a variety of multivariate analysis techniques, such as principal component analysis (PCA), to provide sensitive discrimination between parent molecules based on spectral differences [24, 25]. For example, PCA with ToF-SIMS has been utilized for identifying and classifying a variety of biologically relevant samples such as sugars , lipids [28, 29], proteins [24–26], cell types [28, 30], and decellularized or acellular ECMs [14, 15, 19, 21].
The analysis of monomeric adsorbed protein films with ToF-SIMS has demonstrated that the HV environment can cause structural changes to these proteins . These changes are indicated by spectral features, such as a more pronounced secondary ion yield from hydrophobic residues or a decrease or disappearance in yields from biochemical moieties that are hydrophilic or polar . To prevent denaturation, it has been necessary to provide some mechanism to stabilize and preserve protein structure prior to analysis [23, 26, 31, 32]. The potential sensitivity of proteins to HV denaturation could limit the usefulness of methods such as ToF-SIMS to provide data that are relevant to the in vivo ECM. With this in mind, it is important to elucidate whether any measurable biomechanical or biochemical changes from HV-exposure occur in complex supramolecular protein structures such as collagen fibrils.
Our group has previously developed a model ECM comprised of type I collagen, the most prevalent ECM protein, which self-assembles into matrices of fibrils [12, 33, 34]. These model matrices have a number of desirable properties that include: (i) collagen in a supramolecular structure that is more physiologically relevant than surface-adsorbed protein monomers , (ii) the ability to elicit robust and reproducible cell responses, (iii) excellent optical properties that facilitate quantifying cell response [12, 33, 34], and (iv) the means of systematically perturbing the chemical and/or mechanical properties [8, 11, 36, 37]. These properties, coupled with the fact that collagen type I is the main component of connective tissue [13, 38, 39], make these fibril matrices an ideal model for studying how exposure to a HV environment may affect the physicochemical properties of supramolecular ECM structures. If the mechanical properties or chemistry of unfixed ECM materials are compromised by exposure to a HV environment, then application of techniques such as ToF-SIMS would require cumbersome and complicating preservation methods for maintaining physiologically relevant structures. However, if the affects from HV exposure were immeasurable, this would help to establish confidence in the use of HV methods for analysis of decellularized scaffolds.
Here, we analyze the effect of various treatments on the well-characterized model ECM of collagen type I fibrils to determine if exposure to a HV environment changes the bioactivity of these matrices, and consequently whether changes are due to differences in biochemical or biomechanical interactions. We have previously shown that passive dehydration of the collagen fibril matrices results in significantly increased spreading and proliferation, as well as other response differences, in NIH 3 T3 cells and vascular smooth muscle cells (A10 vSMCs) compared to cells on untreated fibril matrices [8, 12, 34, 40, 41]. The observed changes in cell response are due to mechanical stiffening of the fibril beds resulting from the dehydration process [11, 12], as opposed to changes in integrin ligation [12, 36, 37]. Here, we examine the affect of HV exposure on fibrillar collagen by directly measuring the mechanical properties of the collagen with AFM, and also measuring biological response in the form of cell spreading. Furthermore, we look for differences in ToF-SIMS spectra of HV-treated and passively dehydrated matrices. We also compare HV treatment with low vacuum (LV) treatment, where the results suggest that conditions in slow removal of water may enhance stiffening of the fibrils due to capillary effects.
Certain commercial products are identified in this report to adequately specify the experimental procedure. Such identification does not imply recommendation or endorsement by the National Institute of Standards and Technology, nor does it imply that the materials or equipment identified are necessarily the best available for the purpose.
2.2 Preparation of collagen fibril matrices
Type I collagen fibril matrices, which are composed of beds of ≈ 150 nm diameter fibrils that can extend to about ≈ 600 nm above the surface , were made as previously described [34, 37]. Briefly, acid-stabilized collagen monomer solution (PureCol®, Advanced BioMatrix, Poway, CA) was diluted to 300 μg/mL using phosphate buffered saline (PBS, Invitrogen, Carlsbad, CA) and neutralized with sodium hydroxide (Sigma, St. Louis, MO). The resulting solution was incubated on gold-coated cover slips functionalized with 1-hexadecanethiol (Sigma) . Alternatively, collagen solutions were incubated on 50 mm bacterial-grade polystyrene (PS) dishes (BD Falcon, Franklin Lakes, NJ) . The samples were placed overnight at 37°C to facilitate collagen polymerization and fibril assembly on the surface. Excess collagen in solution was then aspirated from the sample, and the surface-adherent collagen was washed with PBS and de-ionized water. Following the washing steps, the matrices were exposed to a brief stream (10 s to 30 s) of filtered N2 to remove the excess surface water from the fibril surface, which results in the creation of a bed of intersecting collagen fibrils. At this point, the fibril bed created is referred to as an untreated matrix. These matrices were stored in PBS at 4°C until further use . Dehydrated collagen matrices were prepared identically to untreated ones, but prior to storage in PBS, they were left to passively dehydrate for 24 h in a laminar flow hood. After the dehydration step they were then stored in PBS at 4°C until further use. To assess the effect that subsequent LV and HV exposure had on untreated fibrillar matrices, the untreated matrix samples were placed into a vacuum desiccator at 1 kPa to 10 kPa of pressure, or a ToF-SIMS sample chamber at 10-7 Pa to 10-8 Pa, respectively, for approximately 6 h. This time period was chosen because it is approximately the longest time the samples would experience these pressures for a HV-based analysis. On removal from the vacuum environments, the samples were placed in PBS and stored at 4°C until further use. All samples were stored in PBS at 4°C for no more than 36 h before they were analyzed.
2.3 Quantification of cell spreading
A10 rat vascular smooth muscle cells (ATCC (Manassas, VA) were cultured as previously described . Briefly, cells were cultured in DMEM (Dulbecco’s Modified Eagles Medium) obtained from Mediatech (Herndon, VA), supplemented with 10 (v/v) fetal bovine serum, non-essential amino acids, and glutamine at 4 × 10-3 mol/L (all from Gibco Invitrogen, Carlsbad, CA). Cells were maintained on tissue culture-treated polystyrene plates in a humidified incubator maintained at 5% CO2 and 37°C and plated for experiments at a density of 1500 cells/cm2. Cells were incubated on collagen fibril matrices for 24 h then rinsed with PBS, fixed with 4% paraformaldehyde in PBS, and permeabilized with 0.5% Triton X-100 in PBS. The fixed cells were stained with Texas Red maleimide (Sigma) to label the cell body and 4’, 6-diamidino-2-phenylindole (DAPI, Sigma) to label the cell nuclei as described previously . Cells were then imaged on an Olympus IX70 inverted microscope (Olympus America, Melville, NY) equipped with a motorized stage for three dimensional position control, motorized filter wheels, and motorized shutters (Ludl Electronic Products, Hawthorne, NY) and controlled by IP Lab imaging software (BD, Exton, PA). Cell areas were then determined using a custom automated method with the Cell Morphology and Indicator Analysis Program, which is an ImageJ (National Institutes of Health, Bethesda, MD) plugin that thresholds and binarizes the fluorescence image data . Analysis of resulting image data was performed in Excel (Microsoft, Redmond, WA) as described previously [12, 36, 37, 42].
2.4 Atomic force microscopy (AFM) of fibril matrices
AFM of the collagen fibril matrices was performed on a MFP-3D-BIO AFM (Asylum Research, Santa Barbara, CA). All AFM measurements were performed at ambient temperature in PBS solution on collagen fibril beds formed on PS dishes, which behave similarly to fibril beds formed on thiolated Au films . PS dishes were used here as the substrate in order to reduce sample preparation time, and because it is a convenient vessel for solution-phase AFM. This circumvented the need to transfer the samples to a secondary fluid cell, and insured that the samples stayed under buffered solution at all times. Topographical images were taken over 5 μm × 5 μm areas at a resolution of 512 pixels × 512 pixels using intermittent-contact mode at a linear scan rate of 0.18 Hz to 0.3 Hz with silicon nitride probes (k nom = 0.03 N/m, BioLever, Olympus, Tokyo). Force microscopy measurements were carried out using the colloidal probe technique [11, 43], which utilizes a microscale colloidal sphere as the probe tip, thereby allowing for mechanical property measurements over contact areas more similar to cell spread areas. In this study, commercially available AFM cantilevers with a gold colloidal sphere (sQube, Wetzlar, Germany) were used. Calibrating the colloidal probe cantilevers and conducting the force spectroscopy on each of the collagen fibril beds have been described previously . Briefly, the colloidal probe cantilevers were calibrated by (i) determining the deflection sensitivity in air, (ii) measuring the spring constant (k) via the thermal fluctuation method in air, and (iii) adjusting the deflection sensitivity in solution such that k remains constant. Using this approach, k for the cantilevers was determined to be 2.03 N/m and 2.21 N/m for the LV- and HV-exposure studies, respectively. In addition, the radius of the gold colloidal spheres as measured by scanning electron micrographs was determined to be 3.3 μm and 3.4 μm for the LV and HV exposure studies, respectively. AFM force-displacement measurements included both extension of the cantilever towards the collagen fibril beds and retraction of the cantilever away from the collagen fibril beds with a peak load of 5 nN at a displacement rate of 5.7 μm/s. Force-deformation data were derived from the raw force-displacement measurements by subtracting the cantilever deflection. The unloading portions of the force-deformation curves were analyzed using the Johnson, Kendall, and Roberts (JKR) elastic contact model , with the Young’s modulus of the fibril bed and the work of adhesion at the fibril bed-probe tip interface as the fitting parameters. A minimum of 14 force-deformation measurements was taken at different locations for each sample. The mean elastic modulus, with the standard deviation, of each sample is reported.
2.5 ToF-SIMS of collagen fibril matrices
Collagen matrices formed on Au-coated coverslips were analyzed with an IONTOF IV time-of-flight secondary ion mass spectrometer (IONTOF GmbH, Munster, Germany). Positive- and negative-ion mass spectra were acquired using a pulsed 25 keV Bi3 + primary ion source in high current bunched mode, and was rastered randomly over 500 μm × 500 μm areas. Pulsed target current was measured using a Faraday cup and was determined to be 0.04 pA at 10 kHz. Ion dose was kept constant and at < 1012 ions/cm2 for all analyses, and all ions ranging from m/z= 0 to m/z= 1000 were detected in parallel. A flood gun was used for charge compensation. Positive-ion spectra were mass calibrated using the CH3 +, C2H3 +, C3H5 +, and C7H7 + ion fragments before further analysis. Mass calibration of the negative-ion spectra was done using CH-, O-, CN-, and C2H2O- fragments. Minimal spectral features were seen in the negative-ion mode spectra of the matrices, as previously reported for ToF-SIMS analysis of other cellular material (e.g., proteins, lipids, and sugars) [24–29].
2.6 Statistical data analysis
Principal component analysis (PCA) was performed on the positive-ion ToF-SIMS data to elucidate any minor spectral differences between the HV-treated and dehydrated fibrils with minimal bias. A comprehensive description of PCA can be found elsewhere . Limiting PCA of the ToF-SIMS data to only amino acid-related fragments, as was suitable in previously reported studies to discriminate between various protein films [15, 23, 24], could prohibit the identification of glyco-related changes to the surface of the collagen fibrils. Accordingly, all peaks with intensities of at least 100 counts were manually selected. Inorganic-related fragments of Li+, Na+, and K+ were omitted from the spectra, and any spectra with Na+ intensity greater than 1% of the total ion counts were discarded from the analysis [24, 46]. The selected peaks were normalized to the total counts of the all of the selected peaks (average total counts 1.2 × 107 counts ± 0.2 × 107 counts) to account for any differences in secondary ion yields between spectra. The ToF-SIMS data was then arranged in a matrix where the different spectra formed the rows and the individual mass peaks formed the columns. This data matrix was exported to the PLS Toolbox (v.6.2.1 Eigenvector Research, Manson, WA), which was run in MATLAB (v.7.11, MathWorks, Inc., Natick, MA). Lastly, mean-centering the spectra was performed prior to PCA.
3 Results and discussion
3.1 Determining the effect of vacuum exposure on untreated, mechanically compliant collagen fibril matrices
A series of treatments were performed on the collagen matrices prepared as described above. Collagen samples that were immediately stored under PBS at 4°C until further use are referred to as untreated fibril matrices. These have been shown to exhibit mechanical flexibility under the forces imposed by cell spreading and migration . Conversely, passively dehydrated beds of collagen fibrils (referred to as dehydrated fibril matrices) are significantly mechanically stiffer than untreated samples [11, 12]. The effects of two other treatments, exposure of untreated matrices to low vacuum (LV-treated) and high vacuum (HV-treated), were analyzed to understand how these conditions affect the properties of previously compliant fibril matrices.
It has been previously observed that adsorbed monomeric proteins denature under HV conditions (e.g., SIMS analysis chamber) . This denaturation results in analytically detectable differences due to conformational changes that result in a display of different surface chemical moieties compared to films that have been chemically stabilized (e.g., trehalose protected, chemically cross-linking, etc.) [23, 26, 31, 32]. If similar conformational changes occur in supramolecular protein structures as compared to their monomeric counterparts, then HV methods for analyzing materials such as decellularized ECMs may likely result in inaccurate determination of biologically relevant mechanical and chemical information. To examine if supramolecular matrix protein assemblies also require stabilization for accurate HV-based analysis, we studied fibrillar collagen matrices, and evaluated them by the biological response they elicited subsequent to HV exposure.
Measured elastic modulus values of the untreated, dehydrated, and HV-treated collagen fibril matrices.
Fibril Matrix Condition
Elastic Modulus (kPa)
8.1 ± 2.2
35.4 ± 4.9
13.1 ± 3.8
Measured elastic modulus values of the untreated, dehydrated, and LV-treated collagen fibril matrices.
Fibril Matrix Condition
Elastic Modulus (kPa)
11.2 ± 3.7
36.4 ± 4.2
34.7 ± 3.7
3.2 Elucidating ToF-SIMS spectral differences of mechanically modulated collagen fibril matrices
ToF-SIMS is an increasingly popular analytical method for studying decellularized and acellular ECMs [14, 15, 21]. A strength of ToF-SIMS is that it can provide insights into spectral differences that may arise as result from structural changes in ECM samples. We used ToF-SIMS to examine untreated and dehydrated collagen fibril matrices to see if any detectable changes in matrix structure occur as a result of dehydration. The data in Figure 3 and Table 1 establishes that exposure to a HV environment did not significantly affect the mechanical properties of compliant collagen fibril matrices, which corroborates the data in Figure 1 showing that cells did not respond differently to the HV-treated fibrils compared to untreated fibrils. Therefore, ToF-SIMS is an appropriate technique to apply to this question, and we will assume that HV-treated matrices are equivalent to untreated matrices. However, even though we are comparing the ToF-SIMS data from untreated and dehydrated matrices, for the subsequent results shown and discussed we do refer to untreated matrices as HV-treated, because technically they were exposed to HV for ToF-SIMS analysis. It would be disingenuous to call these samples ‘untreated’, even if they retained the same bioactive and mechanical properties.
It is unclear what the observed minor differences in spectra between the HV-treated and dehydrated fibril films are due to. One could speculate that the higher relative abundance of large molecular fragments with greater than m/z≈ 73 in the HV-treated fibril matrices could be due to enhancement from the presence of water within the wrapped rope-like structure of the collagen fibrils that is not removed in the HV environment. However, signal enhancement due to water is typically accompanied by an increased yield of H3O+, which is not present in the positive-ion spectra of the untreated fibril matrices (Figure 6, H3O+ signal is annotated). Alternatively, the spectral differences observed here could be due to topographic differences between the two samples. We have shown here and elsewhere  that the average height of the large fibrils is reduced during the dehydration process, and it has been established previously that PCA can capture topographical differences in the ToF-SIMS data of samples . Another possibility is that our observations are due to the fact that the dehydration process causes the large fibrils to become brittle . Therefore we may expect to see that the mechanically stiff matrices have relatively higher yields in small m/z fragments than in the mechanically compliant matrices. Differences in topography and/or brittleness may also explain why the H− yield in the negative-ion spectrum of the dehydrated fibril matrices (Additional file 1: Figure S1b) is larger than in untreated matrices (Additional file 1: Figure S1a). Regardless of what causes the observed increase of small fragments, the ToF-SIMS results indicate there are no measureable chemical changes at the surface of the fibril matrices due to the dehydration process. This is corroborated by our previous work that found known biochemical cues remain intact between the untreated and dehydrated matrix states [36, 37].
This work demonstrates that unlike their monomeric protein film counterparts [26, 31, 32], collagen type I fibril matrices are not mechanically or biochemically altered by the HV environment. Collagen type I is the primary protein in connective tissue [13, 38, 39], and the supramolecular structures that constitute the fibril matrices in this study are a physiologically relevant configuration of collagen . To the extent that these collagen matrices are similar to the fibrillar structures found in decellularized matrices, these results support the possibility that HV methods can provide accurate information about decellularized ECMs.
5 Supporting information available
Figures illustrating the representative negative-ion spectra of the HV-treated and dehydrated matrices, cell spreading on the ToF-SIMS analyzed samples, and PCA using an amino acid-related peak set of the ToF-SIMS positive-ion spectra of HV-treated and dehydrated fibril matrices. Also, tables summarizing the loading values for each PCA of the positive-ion ToF-SIMS data. This material is available free of charge on the Internet.
The authors would like to thank Dr. Karen T. Henry for assisting in the SEM measurements to determine the radii of the AFM colloidal probes. Furthermore, the authors would like to thank Dr. John T. Elliot, Dr. Christopher Szakal, and Dr. Shin Muramoto for useful discussions. CRA was supported by the National Research Council Associates Program.
- Holly SP, Larson MK, Parise LV: Multiple roles of integrins in cell motility. Exp Cell Res 2000,261(1):69–74.View ArticleGoogle Scholar
- Dallas SL, Chen Q, Sivakumar P: Dynamics of assembly and reorganization of extracellular matrix proteins. Curr Top Dev Biol 2006, 75:1–24. http://www.ncbi.nlm.nih.gov/pubmed/16984808 View ArticleGoogle Scholar
- Roskelley CD, Bissell MJ: The dominance of the microenvironment in breast and ovarian cancer. Semin Cancer Biol 2002,12(2):97–104.View ArticleGoogle Scholar
- McCloskey KE, Gilroy ME, Nerem RM: Use of embryonic stem cell-derived endothelial cells as a cell source to generate vessel structures in vitro. Tissue Eng 2005,11(3–4):497–505.View ArticleGoogle Scholar
- Mercier I, Lechaire J-P, Desmouliere A, Fo G, Aumailley M: Interactions of human skin fibroblasts with monomeric or fibrillar collagens induce different organization of the cytoskeleton. Exp Cell Res 1996,225(2):245–256.View ArticleGoogle Scholar
- Hynes RO: Integrins: bidirectional, allosteric signaling machines. Cell 2002,110(6):673–687.View ArticleGoogle Scholar
- Lo C-M, Wang H-B, Dembo M, Y-l W: Cell movement is guided by the rigidity of the substrate. Biophys J 2000,79(1):144–152.View ArticleGoogle Scholar
- Plant AL, Bhadriraju K, Spurlin TA, Elliott JT: Cell response to matrix mechanics: focus on collagen. BBA-Mol Cell Res 2009,1793(5):893–902.Google Scholar
- Lathia JD, Rich JN: Holding on to stemness. Nat Cell Biol 2012,14(5):450–452.View ArticleGoogle Scholar
- Trappmann B, Gautrot JE, Connelly JT, Strange DGT, Li Y, Oyen ML, Cohen Stuart MA, Boehm H, Li B, Vogel V, Spatz JP, Watt FM, Huck WTS: Extracellular-matrix tethering regulates stem-cell fate. Nat Mater 2012,11(7):642–649.View ArticleGoogle Scholar
- Chung K-H, Bhadriraju K, Spurlin TA, Cook RF, Plant AL: Nanomechanical properties of thin films of type I collagen fibrils. Langmuir 2010,26(5):3629–3636.View ArticleGoogle Scholar
- McDaniel DP, Shaw GA, Elliott JT, Bhadriraju K, Meuse C, Chung K-H, Plant AL: The stiffness of collagen fibrils influences vascular smooth muscle cell phenotype. Biophys J 2007,92(5):1759–1769.View ArticleGoogle Scholar
- Badylak SF, Freytes DO, Gilbert TW: Extracellular matrix as a biological scaffold material: structure and function. Acta Biomater 2009,5(1):1–13.View ArticleGoogle Scholar
- Barnes CA, Brison J, Michel R, Brown BN, Castner DG, Badylak SF, Ratner BD: The surface molecular functionality of decellularized extracellular matrices. Biomaterials 2011,32(1):137–143.View ArticleGoogle Scholar
- Canavan HE, Graham DJ, Cheng X, Ratner BD, Castner DG: Comparison of native extracellular matrix with adsorbed protein films using secondary ion mass spectrometry‚Ä†. Langmuir 2006,23(1):50–56.View ArticleGoogle Scholar
- Yeung T, Georges PC, Flanagan LA, Marg B, Ortiz M, Funaki M, Zahir N, Ming W, Weaver V, Janmey PA: Effects of substrate stiffness on cell morphology, cytoskeletal structure, and adhesion. Cell Motil Cytoskel 2005,60(1):24–34.View ArticleGoogle Scholar
- Gilbert TW, Sellaro TL, Badylak SF: Decellularization of tissues and organs. Biomaterials 2006,27(19):3675–3683.Google Scholar
- Hsiao Y-C, Lee H-W, Chen Y-T, Young T-H, Yang T-L: The impact of compositional topography of amniotic membrane scaffold on tissue morphogenesis of salivary gland. Biomaterials 2011,32(19):4424–4432.View ArticleGoogle Scholar
- Canavan HE, Cheng X, Graham DJ, Ratner BD, Castner DG: Surface characterization of the extracellular matrix remaining after cell detachment from a thermoresponsive polymer. Langmuir 2004,21(5):1949–1955.View ArticleGoogle Scholar
- Ott HC, Matthiesen TS, Goh S-K, Black LD, Kren SM, Netoff TI, Taylor DA: Perfusion-decellularized matrix: using nature's platform to engineer a bioartificial heart. Nat Med 2008,14(2):213–221.View ArticleGoogle Scholar
- Brown BN, Barnes CA, Kasick RT, Michel R, Gilbert TW, Beer-Stolz D, Castner DG, Ratner BD, Badylak SF: Surface characterization of extracellular matrix scaffolds. Biomaterials 2010,31(3):428–437.View ArticleGoogle Scholar
- Klerk LA, Dankers PYW, Popa ER, Bosman AW, Sanders ME, Reedquist KA, Heeren RMA: TOF-secondary Ion mass spectrometry imaging of polymeric scaffolds with surrounding tissue after in vivo implantation. Anal Chem 2010,82(11):4337–4343.View ArticleGoogle Scholar
- Baugh L, Weidner T, Baio JE, Nguyen P-CT, Gamble LJ, Stayton PS, Castner DG: Probing the orientation of surface-immobilized protein G B1 using ToF-SIMS, sum frequency generation, and NEXAFS spectroscopy. Langmuir 2010,26(21):16434–16441.View ArticleGoogle Scholar
- Wagner MS, Castner DG: Characterization of adsorbed protein films by time-of-flight secondary ion mass spectrometry with principal component analysis. Langmuir 2001, 17:4649–4660.View ArticleGoogle Scholar
- Wagner MS, Tyler BJ, Castner DG: Interpretation of static time-of-flight secondary ion mass spectra of adsorbed protein films by multivariate pattern recognition. Anal Chem 2002, 74:1824–1835.View ArticleGoogle Scholar
- Xia N, May CJ, McArthur SL, Castner DG: Time-of-flight secondary Ion mass spectrometry analysis of conformational changes in adsorbed protein films. Langmuir 2002,18(10):4090–4097.View ArticleGoogle Scholar
- Berman ESF, Kulp KS, Knize MG, Wu L, Nelson EJ, Nelson DO, Wu KJ: Distinguishing monosaccharide stereo- and structural isomers with TOF-SIMS and multivariate statistical analysis. Anal Chem 2006,78(18):6497–6503.View ArticleGoogle Scholar
- Anderton CR, Vaezian B, Lou K, Frisz JF, Kraft ML: Identification of a lipid-related peak set to enhance the interpretation of TOF-SIMS data from model and cellular membranes. Surf Interface Anal 2011,44(3):322–333.View ArticleGoogle Scholar
- Vaezian B, Anderton CR, Kraft ML: Discriminating and imaging different phosphatidylcholine species within phase-separated model membranes by principal component analysis of TOF-secondary Ion mass spectrometry images. Anal Chem 2010,82(24):10006–10014.View ArticleGoogle Scholar
- Kulp KS, Berman ESF, Knize MG, Shattuck DL, Nelson EJ, Wu L, Montgomery JL, Felton JS, Wu KJ: Chemical and biological differentiation of three human breast cancer cell types using time-of-flight secondary Ion mass spectrometry. Anal Chem 2006,78(11):3651–3658.View ArticleGoogle Scholar
- Xia N, Castner DG: Preserving the structure of adsorbed protein films for time-of-flight secondary ion mass spectrometry analysis. J Biomed Mater Res A 2003,67A(1):179–190.View ArticleGoogle Scholar
- Xia N, Shumaker-Parry JS, Zareie MH, Campbell CT, Castner DG: A streptavidin linker layer that functions after drying. Langmuir 2004,20(9):3710–3716.View ArticleGoogle Scholar
- Elliott JT, Halter M, Plant AL, Woodward JT, Langenbach KJ, Tona A: Evaluating the performance of fibrillar collagen films formed at polystyrene surfaces as cell culture substrates. Biointerphases 2008,3(2):19–28.View ArticleGoogle Scholar
- Elliott JT, Tona A, Woodward JT, Jones PL, Plant AL: Thin films of collagen affect smooth muscle cell morphology. Langmuir 2003,19(5):1506–1514.View ArticleGoogle Scholar
- Meshel AS, Wei Q, Adelstein RS, Sheetz MP: Basic mechanism of three-dimensional collagen fibre transport by fibroblasts. Nat Cell Biol 2005,7(2):157–164.View ArticleGoogle Scholar
- Bhadriraju K, Chung K-H, Spurlin TA, Haynes RJ, Elliott JT, Plant AL: The relative roles of collagen adhesive receptor DDR2 activation and matrix stiffness on the downregulation of focal adhesion kinase in vascular smooth muscle cells. Biomaterials 2009,30(35):6687–6694.View ArticleGoogle Scholar
- Spurlin TA, Bhadriraju K, Chung K-H, Tona A, Plant AL: The treatment of collagen fibrils by tissue transglutaminase to promote vascular smooth muscle cell contractile signaling. Biomaterials 2009,30(29):5486–5496.View ArticleGoogle Scholar
- Di Lullo GA, Sweeney SM, Korkko J, Ala-Kokko L, San Antonio JD: Mapping the ligand-binding sites and disease-associated mutations on the most abundant protein in the human, type I collagen. J Biol Chem 2002,277(6):4223–4231.View ArticleGoogle Scholar
- Nimni ME: Collagen. CRC, Boca Raton, FL; 1988. http://www.amazon.com/Collagen-Biochemistry-Vol-Marcel-Nimni/dp/0849346010 Google Scholar
- Elliott JT, Woodward JT, Langenbach KJ, Tona A, Jones PL, Plant AL: Vascular smooth muscle cell response on thin films of collagen. Matrix Biol 2005,24(7):489–502.View ArticleGoogle Scholar
- Langenbach K, Elliott J, Tona A, McDaniel D, Plant A: Thin films of type 1 collagen for cell by cell analysis of morphology and tenascin-C promoter activity. BMC Biotechnol 2006,6(1):14.View ArticleGoogle Scholar
- Elliott JT, Tona A, Plant AL: Comparison of reagents for shape analysis of fixed cells by automated fluorescence microscopy. Cytometry A 2003,52A(2):90–100.View ArticleGoogle Scholar
- Ducker WA, Senden TJ, Pashley RM: Direct measurement of colloidal forces using an atomic force microscope. Nature 1991,353(6341):239–241.View ArticleGoogle Scholar
- Johnson KL, Kendall K, Roberts AD: Surface Energy and the Contact of Elastic Solids. Proc London R Soc A-Math Phys Eng Sci 1971,324(1558):301–313.View ArticleGoogle Scholar
- Wold S: Principal component analysis. Chemom Intell Lab Syst 1987, 2:37–52.View ArticleGoogle Scholar
- Oran U, Unveren E, Wirth T, Unger WES: Poly-dimethyl-siloxame (PDMS) contamination of polystyrene (PS) oligomers samples: a comparison of time-of-flight static secondary ion mass spectrometry (TOF-SSIMS) and X-ray photoelectron spectroscopy (XPS) results. Appl Sur Sci 2004, 227:318–324.View ArticleGoogle Scholar
- Rosenblatt J, Devereux B, Wallace DG: Injectable collagen as a pH-sensitive hydrogel. Biomaterials 1994,15(12):985–995.View ArticleGoogle Scholar
- Szakal C, Narayan K, Fu J, Lefman J, Subramaniam S: Compositional mapping of the surface and interior of mammalian cells at submicrometer resolution. Anal Chem 2011,83(4):1207–1213.View ArticleGoogle Scholar
- Duan H, Berggren KK: Directed self-assembly at the 10 nm scale by using capillary force-induced nanocohesion. Nano Lett 2010,10(9):3710–3716.View ArticleGoogle Scholar
- Jeon S, Park J-U, Cirelli R, Yang S, Heitzman CE, Braun PV, Kenis PJA, Rogers JA: Fabricating complex three-dimensional nanostructures with high-resolution conformable phase masks. Proc Natl Acad Sci USA 2004,101(34):12428–12433.View ArticleGoogle Scholar
- Chandra S: Challenges of biological sample preparation for SIMS imaging of elements and molecules at subcellular resolution. Appl Surf Sci 2008,255(4):1273–1284.View ArticleGoogle Scholar
- Pachuta SJ: Enhancing and automating TOF-SIMS data interpretation using principal component analysis. Appl Sur Sci 2004, 231–232:217–223.View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.